EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES


 Valentine Payne
 1 years ago
 Views:
Transcription
1 EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510
2 EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLY WOOD CONSIDERED AS ORTHOTROPIC MATERIALS 1 By Forest Products Laboratory, 2 Forest Service U. S. Department of Agiculture Abstract This is a mathematical analysis of the stress distribution existing near a hole in a wood or plywood plate subjected to tension, as, for example, near holes in the tension flanges of wood box beams. It is assumed that the strains are small and remain within the proportional. limit. In this analysis a large, rectangular, orthotropic plate with a small, elliptic hole at the center is subjected to a uniform tension along two opposite edger. By taking equal axes for the elliptic hole, the theoretical stress distribution in the neighborhood of a circular hole is obtained. The analysis shows that for a circular hole in a plainsawn plate of Sitka spruce a maximum tensile stress of 5.84S is attained, S being the uniform tension applied in the direction of the grain. This maximum stress occurs on the edge of the circular hole at the ends of the diameter parpendicular to the direction of the uniform tension. Although this stress concentration may be greater than that found in isotropic materials, it is much more sharply localized and is relieved by plastic flow when the stress exceeds the proportional limit. For the reader who does not wish to follow the mathematical details of this report, the formula for computing this maximum stress for wood or plywood and an explanation of the constants involved is given in the appendix. The formula has not 1 This progress report was originally preparted by the Forest Products Laboratory in Maintained at Madison, Wis., in cooperation with the University of Wisconsin. Report No AgricultureMadison
3 been confirmed by an extensive series of tests, but it was found to be in reasonably satisfactory agreement with the only test made. It is also demonstrated that for the Sitka spruce plate mentioned the maximum shear stress attained is 0.71S (fig. 5). The stress function from which these formulas for the orthotropic case are obtained is shown to reduce to the wellknown stress function for the isotropic case. Introduction An orthotropic material possesses three planes of elastic symmetry at right angles to each other. If from such a material a flat plate is cut parallel to a plane of symmetry, it will have two perpendicular axes of symmetry in the plane of the plate. In the discussion that follows, a large rectangular orthotropic plate of this type with its edges parallel to the axes of symmetry and with a small hole at its center will be considered. A uniform tension S will be taken to act on two opposite edges of the plate as shown in figure 1, and the resulting stress distribution will be obtained. Throughout the report it is assumed that the strains are small and remain within the limits of "perfect elasticity." The solution is first derived for an elliptic hole with major and minor axes coinciding with the axes of symmetry. By taking the major and minor axes equal, the solution for a circular hole is obtained. For the orthotropic plate, the solution for the circular hole is but slightly more simple than that for the elliptic hole. This is different from the corresponding problem for the isotropic plate. 3 The stressstrain distribution in the neighborhood of the circular hole is notably different in an orthotropic plate than in an isotropic plate as the concentration may be considerably higher and of a more localized character for the orthotropic than for the isotropic plate. Thus in a plate of plainsawn Sitka spruce with a uniform tension acting in the grain direction, the greatest stress component at the edge of the hole decreases rapidly to onehalf of its maximum value in a radial distance of less than onetenth of the radius. For the isotropic plate the corresponding stress component decreases to onehalf of its maximum value in a radial distance larger than onehalf of the radius from the edge of the hole. 3 Timoshenko, S. Theory of Elasticity. Report No
4 The Effect of Eliptic or Circular Holes on the Stress Distribution in a Wood Plate The components of stress and strain in a plate under plane stress are connected by the following relations 4 if the axes of x and y are taken as the axes of elastic symmetry of the orthotropic plate: (1) In these equations E x and E y are Young's moduli in the x and y directions, respectively. Poisson's ratio σ xy is the ratio of the contraction parallel to the y axis to the extension parallel to the x axis associated with a tension parallel. to the x axis and similarly for σ yx. The quantity µ xy is the modulus of rigidity associated with the directions of x and y. Since the equations of equilibrium are deduced with no reference to the law connecting stresses and strainns, they will be satisfied by a stress function F such that (2) 4 March, H.W., StressStrain Relations in Wood and Plywood Considered as Orthotropic Materials, U. S. Forest Products Laboratory Report No Report No
5 Substituting (2) in (1) and then making use of the compatibility equation the following differential equation, obtained: satisfied by the stress function F, is (3) In deriving (3), the relation 4 (4) has been used. It is convenient to rewrite equation (3) as 5 (5) where (6) by making the substitution (7) 5 March, H, W., Flat Plates of Plywood Under Uniform or Concentrated Loads, U. S. Forest Products Laboratory Report No Report No,
6 where (8) Substituting F = F(x + vη) in (5) leads to the following equation for v: (9) or Now let 6 (10) (11) then 6 For wood or plywood, k as defined here is probably always greater than 1. Report No
7 Hence, the roots of equation (9) are Equation (5) may now be written as (12) where (13) The solution of equation (13) is facilitated by taking F of the form (14) where (15) F o ( x, η ) is any particular solution of (12), and the letter R means that the real part of the expression in the bracket is to be taken. That (14) is a solution of (12) is easily established by direct substitution. Equations (12) and (14) hold for the stress function associated with any elastic problem of plane stress in an orthotropic plate with x and y axes chosen as described here. Report No
8 A suitable choice of F for the problem discussed is (16) where (17) (18) the boundary of the hole (fig. 1) is given by (19) and S is the uniform tension applied at the ends of the plate. In order that the stresses may be singlevalued, the square roots in (17) are to be chosen so that the following relations always hold: Report No
9 Then (20) and (21) On the boundary of the hole x and η are given by (19), so that (22) (23) Similarly, on the edge of the hole (24) Consider the boundary of the hole in figure 2, and orient the positive direction of the normal v and of the tangent τ relative to one another in a way similar to the orientation of the x and yaxis, respectively. Report No
10 Let X v ds and Y v ds represent and x  and y components of the force per unit thickness of the plate, acting on the element of arc ds of the boundary from the positive side indicated by the direction of positive v. Then But (25) so that (26) Report No
11 Equations (26) for a boundary on which no stresses act take the form Hence, and are constant along a free boundry. Then, on the boundary of the hole, (27) Substituting (23) and (24) in (20) and (21), it follows from (27) that and (28) Taking the real parts (29) These equations must be satisfied for any value of θ, hence Report No
12 and Therefore, (30) By using equations (30), the stress components are found to be (31) (32) (33) To obtain the stress components for a circular hole, it is only necessary to let b = a in equations (31), (32), and (33). Then Report No
13 (34) (35) (36) where (37) Expressions (31), (32), (33) are complicated and do not permit easy computation of the numerical values of the stresses. The most important information they contain is, of course, in the neighborhood of the hole. Stresses at the Edge of the Hole From equations (22), (23), and (24), it is found that over the edge of the elliptic hole Report No
14 (40) Since, by (15) αβ = 1, the real parts are given by (41) (42) (43) where (44) It is of interest to refer these stresses at the edge of the hole to a pair of axes at right angles to each other having the directions of the normal v and the tangent τ, respectively (fig. 2). In this coordinate system, the shearing stress and the tension (or compression) in the vdirection must vanish, as this is required by the boundary conditions. It is readily shown that T τ of equation (44) is the tension (or compression) in the tangential direction. The component of direct stress in the tangential direction is given by Report No
15 From (19) and (25), this becomes Substituting from (41), (42), and (43), the tangential stress is found to be identical with T t of equation (44). If ε 1, it follows that at the end of the axis perpendicular to the direction of the tension, that is for θ = 90 (fig. 1), T τ attains its maximum value, while at the end of the axis parallel to the tension, that is θ = 0, T τ attains its minimum value. Then (45a) (46) For an isotropic material, it follows from (6), (8), (11), and (15) that α = β = ε = 1. Introducing these values, (45a) and (46) become S( 2b + 1) a and S, respectively, as in the isotropic case. 3 Equation (45a) gives the tension at C (fig. 1) the highest stress occurring in the plate. Numerical values of this stress will be computed in the two cases b 1 a = 50 and b a = for a plainsawn plate of Sitka spruce whose 50 elastic moduli are given in table 1. The grain direction is taken parallel to the line θ = 0. When b = 50, the tension at C (fig. 1) is times the mean tension. a When b = 1, the tension at C (fig. 1) is times the mean tension. a 50 Report No
16 The ellipse when b a = 50 would appear as a straight crack perpendicular to the grain which might be approximated by a break in the fibers, such as a compression failure. A very small tension applied to the plate across the crack would set up a tension at the ends of very high intensity. If this high tension at the ends caused the crack to tear, the increase in length would exaggerate the stress still further, and the crack would continue to spread. When b = 1 the ellipse would appear as a straight crack running in the a 50 direction of the grain or of the tension. Such a crack does not produce great local stress, a conclusion which is almost selfevident. If the hole is circular ( b = 1), equations (41), (42), (43), and (44) reduce to a where The stress at the end of the diameter perpendicular to the direction of the tension for a circular hole is given by (45b) For an isotropic plate ( α = β = ε =1) this reduces to 3S, as is well known, 3 but for a wood plate, equation (45b) may give a stress as high as 5.84S (fig. 8). Report No
17 Experimental Verification of Maximum Stress This maximum stress was experimentally verified by compressing a quartersawn yellowpoplar board containing a circular hole. The dimensions of the board and hole and the position of the 1/8inch metalectric strain gages at P on the circumference of the hole and at Q at some distance from the hole are shown in figure 3. The gage measuring the maximum strain at P was placed inside the hole as shown in figure 3, since the maximum strain occurs just on the edge of the hole and dies off rapidly in the radial direction. The gage at Q is placed as far from the hole as is feasible for the specimen used. The gage length was assumed short enough to give a close approximation to the actual strain at the end of the diameter. Table 2 gives the experimental and the theoretical values of the strains at pints P and Q of figure 3. The theoretical strains were computed in terms of S from the stresses given by formulas (35) and (45b) using the elastic moduli of the yellowpoplar plate. These moduli were obtained from coupons cut from the specimen and are given in table 1. The experimental value of the ratio of the strain at P to the strain at Q (fig. 3) is about 16 percent less than the theoretical one. This difference is not considered serious as the mathematical analysis was based on the assumption that the dimensions of the plate were large as compared to the dimensions of the hole. Also the impossibility of measuring strain at a point acted to decrease the apparent ratio. It is important to note that the experimental ratio is considerably higher than the corresponding ratio existing for a circular hole in an isotropic plate. Shear Stress at the Edge of the Hole The expression (43) for the shear component at the edge of the hole is highly important when considering holes in wood plates. When the uniform tension is parrallel to the grain direction, this shear acts in the same direction, and its distribution may indicate where failure caused by shear will take place if the uniform tension is sufficiently high. This statement has experimental verification when b = 1, as this type of faila ure occurred in wood box beams with small circular holes in their tension flanges tested at the U. S. Forest Products Laboratory (see fig. 4), The failure occurred in the vicinity of the point of maximum shear, which occurs theoretically, as shown in figure 5, at about θ = 78. The shear stress at the edge of the hole was evaluated numerically when b a = 1 for a plainsawn plate of Sitka spruce whose elastic moduli are given in Report No
18 table 1. The results are given in table 3 for values of θ between 0 and 90 when the line θ = 0 is taken to be parallel to the grain of the wood. The shear at other points on the circle may be easily filled in from the given values. Figure 5 illustrates the variation of X y over the edge of the hole for spruce and an isotropic material. Stress Components at Points Along the x and yaxes Simple expressions will now be obtained for the stress components at points along the x and yaxes. Writing equation (31) as and performing similar operations on equation (32) and (33), it is found that (47) These equations can be reduced considerably when x = 0 or y = 0. The resulting equations then readily show how the stress concentration dies off with increasing distance from the hole. Report No
19 > For x = 0, y = a it follows that (48) > a and for y = 0, x = (49) When b a = 1 the distances from the center of the hole may be expressed as multiples of the radius by writing x 1 = x a, y 1 = y in equations (48) and (49). Hence, the a stress components at points along the positive yaxis for a circular hole are given by Report No
20 (50) and at points along the positive xaxis (51) Numerical values of the stress components X x and Y y at points along the x and y axis when b = 1 are given in tables 4 and 5 for a plainsawn plate of Sitka spruce. a The variation of these components is illustrated in figures 6, 7, 8, and 9, and the variation of the corresponding stress components for an isotropic material is also shown for comparison. It is evident from these figures that considerable differ ences may exist between the stress distribution developed in the orthotropic plate as compared to the isotropic plate. In particular, figure 8 shows that the maximum stress developed in the spruce plate is nearly twice the maximum stress developed in the isotropic plate. Report No
21 Displacements in the Neighborhood of a Circular Hole The expressions for the displacements in the neighborhood of a circular hole ( b = 1) will now be obtained. a Substituting (34) and (35) in the first two equations of (1), it is found that (52) Integration of equations (52), gives Report No
22 (53) These are the actual displacements except for the addition of a linear function of y and a linear function of x to the expressions for u and v, respectively. This is easily shown by deriving the expression for e xy = + and comparing it with the expression These additive functions may be made rotation about the origin. to vanish by fixing the origin and eliminating Next the real and imaginary parts of and of a similar expression for z 2 and w 2 will be found. TO do this, it will be useful to write Let (54) where Report No (55)
23 (56) Then (57) Similarly (58) where (59) (60) To keep the displacements singlevalued, Y 1 and Y 2 must always be taken so that the following relations hold: Report No
24 Taking the real parts, equations (53) become (61) (62) These equations for the displacements would be used to check data given by strain gages of finite length, since the strains computed from the gage readings are average strains. Isotropic Stress Function as the Limiting Case of the Orthotropic Stress Function It is of interest to obtain from (16) the stress function for the corresponding problem when b = 1 for an isotropic material. a Substituting from (15) and (30), (16) becomes Report No
25 (63) For an isotropic material φ becomes equal to 0, and α, β, and ε each becomes equal to unity as sh own by equations (6), (8), (11), and (15). For these values, parts of equation (63) take the indeterminate form 0 0. Evaluating by differentiating both numerator and denominator with respect to φ (remembering that z 1, x 2, γ 1, and γ 2 all contain φ ), It follows that Report No
26 Report No
27 Let φ = 0 and ε = 1. Then (64) takes the form (65) where On setting b = a, parts of equation (65) assume the indeterminate form 0. On evaluating (65), it is found that for the circular hole, 0 (66) (67) Since the constant 2a 2 log 2 will not appear in the stresses obtained from (67), it may be omitted. The real. part of (67) is in polar form: (68) Report No
28 which is the wellknown form for the stress function in the corresponding problem for the isotropic plate.3 The Effect of Elliptic or Circular Holes on_. the Stress Distribution in a Plywood Plate A plywood panel having the grain direction of each ply perpendicular to that of the adjacent plies and having a symmetrical construction may be considered as an orthotropic plate. The strains in such plywood may be obtained from the average stresses (to be defined later), or the average stresses from the strains, 4 by exactly the same relations as exist between the strains and stresses for an orthotropic plate if the apparent elastic moduli of the plywood are used as the elastic moduli of the orthotropic plate. The panel is assumed to remain flat under the application of the loading considered. The xaxis will be taken parallel to the grain direction of the face plies. The subscript 1 will be used to denote quantities associated with plies having grain direction parallel to the xaxis, and the subscript 2 will be used to denote quantities associated with plies having grain direction parallel to the yaxis. Let h 1 denote the total thickness of all plies having grain direction parallel. to the xaxis. Let h 2 denote the total thickness of all plies having grain direction parallel to the yaxis, For plies having grain direction parallel to the xaxis, the following relations hold (69) Report No
29 and for plies having grain direction parallel to the yaxis corrosponding equations hold if the subscripts are changed. Since the panel remains flat, it will be assumed that (e xx ) 1 = (e xx ) 2. (e yy ) 1 = (e yy ) 2, (e xy ) 1 = (e xy ) 2, and it is no longer necessary to write the strain components with subscripts. Solving equations (69) for the stress components gives (70) where Similar relations hold in the remaining plies if the subscripts are changed throughout. Assuming the plies are all rotary cut and from the choice of axes, the elastic constants have the following values in the respective plies: Report No
30 After making these changes, equations (70) become (71) where Report NO
31 It is now important to define the mean stress components X x and Y y by the following equations: (72) where h = h 1 + h 2, the overall thickness of the plywood, and the relation ham been used. Equations (72) may be rewritten as follows: (73) where (74) Report No
32 Solving equations (73) for the strain components gives or (75) where 7 (76) It is easily established that 7 Since σ xy, σ xy, etc. are usually small, E x and E y are approximately equal to E a and E b, respectively. Report No
33 In plies with grain direction parallel to the xaxis, the conditions of equilibrium require and similarly in the remaining plies Then (77) (78) and Report No
34 (79) (80) Adding equations (77) and (79) and dividing by h, it is found that (81) where, since in all plies the relation holds, the mean stress component X y is identical with the stress component X y. Similarly equation (78) and (80) yield (82) Equations (81) and (82) will be satisfied by a stress function F, such that (83) Substituting (83) in (75) and then making use of the compatibility equation Report No
35 the following differential equation satisfied by the stress function F is found: As in the treatment of equation (3), it will be convenient to rewrite this equation as (84) where (85) by making the substitution where (86) (87) The differential equations (84) and (5) are of the same form mathematically, and any solution of (5) is a solution of (84) if the appropriate constants are used. It is then possible by using equations (31), (32), and (33) to obtain the stress distribution in the neighborhood of an elliptic hole situated in the middle of a plywood plate subjected to a uniform tension, provided that the axes of the ellipse are parallel and perpendicular to the grain of the face plies and that the tension is applied parallel or perpendicular to the axes of the ellipse. Report No
36 Hence, if the K and ε calculated from the apparent clastic: moduli of plywood are used, all of the preceding discussion for orthotropic plates containing elliptic holes holds for plywood panels. Numerical values for the stresses at various points along the x and y axes in the case b = 1 for rotarycut Sitka spruce plywood having half a the material with grain direction parallel to the xaxis are given in tables 6 and 7. Figures 10, 11, 12, and 13 illustrate how these stresses vary in the neighborhood of the hole. The foregoing analysis for plywood is based on the assumption that all plies are rotary cut and of the same species of wood. When these assumptions are not fulfilled, it is easy to make suitable modifications in the analysis (see appendix). Report No
37 Appendix A plainsawn or a quartersawn wood plate ox a plywood plate may be considered to have two perpendicular axes of elastic symmetry in the plane of the plate. The discussion given in this appendix applies to a rectangular plate of this type with its edges parallel to the axes of symmetry and with a small circular hole at the center. The x and yaxes are taken as the axes of symmetry. A uniform tension S directed parallel to the xaxis is supposed to act on the two opposite edges of the plate, and the tensile stress on the edge of the hole at the end of the diameter perpendicular to the uniform tension is given by For wood, the constants that appear in this expression are defined a3 follows: ε α β e = natural logarithmic base E x = Young's modulus in the xdirection E y = Young's modulus in the ydirection µ xy = modulus of rigidity In the xyplane Report No
38 σ xy = the Poisson's ratio given by the ratio of the contraction parallel to the yaxis to the extension parallel to the x axis associated with a tension parallel to the xaxis. For plywood, equations similar to those already given for wood define ε, α, β, φ, and K if the remaining constants are as subsequently defined. The plies will be considered to be numbered consecutively from the upper to the lower face. The elastic moduli in the ith ply will be denoted by (E x ) i, (E y ) i, (µ xy ) i, and (σ xy ) i. The thickness of the ith ply is h i. That of the plate is h. Then approximately 4 The shear parallel or perpendicular to direction of the uniform tension and on the edge of the circular hole is given in the mathematical part of the report by equation (43) if b is set equal to a. By substituting the constants defined previously, this shear stress may be plotted as a function of the polar coordinate θ (fig. 5), and its maximum value read from the curve. Report No
39 Table 1. Elastic moduli of Sitka spruce and yellow popular 1 Species Sitka spruce Yellowpoplar 1 The elastic moduli of Sitka spruce are average values obtained from a large number of tests made at the U.S. Forest Products Laboratory. The elastic moduli of yellowpoplar are values obtained from the one specimen used in the experimental verification of this report. 2 Not used. Table 2. Observed and theoretical values of the strains at the points P and Q of figure 3 Type Strain at P Strain at Q Ratio of strain at P to strain at Q Observed Theoretical (computed from equations (35) and (45b)) Inch per inch Report No. 1510
40 Report No. 1510
41 Table 4. Values of the stress components at points along the xaxis exterior to a circle of radius a and with center at the origin for a plainsawn plate of Sitka spruce  Report No. 1510
42 Report No Table 5. Values of the stress components at points along the y axis exterior to a circle of radius a and with center at the origin for a plainsawn plate of Sitka spruce
43 Table 6. Values of the stress components at points along the xaxis exterior to a circle of radius a and with center at the origin for a rotarycut plywood plate of Sitka spruce Table values of the stress components at points along the yaxis exterior to a circle of radius a and with center at the origin for a rotarycut plywood plate of Sitka spruce Report No. 1510
44 Figure 1Elliptic hole in orthotropic plate. Figure 2.Orientationof positive normal and tangent on the boundary of the elliptic hole. Z M F
45 Figure 3.Circular hole in a quartersawn yellowpoplar board subjected to a uniform compression. Z M F
46 Figure 4.The tension flange of a loaded wood box beam showing shear failure caused by vertical holes. The beam is subjected to a lower load in A than in B. The small cracks occurred in the stresscoat, which was applied to the beam before testing. The small round objects paralleling the edge of the flange are Whittemore strain gage points. Z M F
47 Z M F Figure 6.Variation of the normal stress component χx at points along the xaxis exterior to a circular hole of radius a and with center at the origin for a plainsawn plate of Sitka spruce and for an isotropic plate.
48 Figure 7.Variation of the normal stress component Yy at points along the xaxis exterior to a circular hole of radius a and with center at the origin for a plainsawn plate of Sitka spruce and for an isotropic plate. ZM F
49 Figure 8.Variationof the normal stress component Xx at points along the yaxis exterior to a circular hole of radius a and with center at the origin for a plainsawn plate of Sitka spruce and for an isotropic plate. Z M F
50 Figure 9.Variation of the normal stress component Y y at points along the y axis exterior to a circular hole of radius a and with center at the origin for a plainsawn plate of Sitka spruce and for an isotropic plate. Z M F
51 Figure 11.Variation of the normal stress component Yy at points along the xaxis exterior to a cir cular hole of radius a and with center at the originfor a rotarycut plywood plate of Sitka spruce. Figure 10.Variation of the normal stress component Xx at points along the xaxis exterior to a circular hole of radius a with center at the origin for a rotarycut plywood plate of Sitka spruce Z M F
52 Figure 12.Variation of the normal stress component Xx at points along the yaxis exterior to a circular hole of radius a and with center at the origin for a rotarycut plywood plate of Sitka spruce. Figure 13.Variation of the normal stress component Yy at points along the yaxis exterior to a circular hole of radius a and with center at the origin for a rotarycut plywood plate of Sitka spruce. Z M F
STRESSES WITHIN CURVED LAMINATED BEAMS OF DOUGLASFIR
UNITED STATES DEPARTMENT OF AGRICULTURE. FOREST SERVICE  FOREST PRODUCTS LABORATORY  MADISON, WIS. STRESSES WITHIN CURVED LAMINATED BEAMS OF DOUGLASFIR NOVEMBER 1963 FPL020 STRESSES WITHIN CURVED LAMINATED
More informationRELATIONSHIP BETWEEN RADIAL COMPRESSIVE MODULUS OF ELASTICITY AND SHEAR MODULUS OF WOOD Jen Y. Liu Research Engineer
RELATIONSHIP BETWEEN RADIAL COMPRESSIVE MODULUS OF ELASTICITY AND SHEAR MODULUS OF WOOD Jen Y. Liu Research Engineer and Robert J. Ross Supervisory Research Engineer USDA Forest Service Forest Products
More informationMechanical Properties of Materials
Mechanical Properties of Materials Strains Material Model Stresses Learning objectives Understand the qualitative and quantitative description of mechanical properties of materials. Learn the logic of
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationLaminated Beams of Isotropic or Orthotropic Materials Subjected to Temperature Change
United States Department of Agriculture Forest Service Forest Products Laboratory Research Paper FPL 375 June 1980 Laminated Beams of Isotropic or Orthotropic Materials Subjected to Temperature Change
More informationBUCKLING COEFFICIENTS FOR SIMPLY SUPPORTED, FLAT, RECTANGULAR SANDWICH PANELS UNDER BIAXIAL COMPRESSION
U. S. FOREST SERVICE RESEARCH PAPER FPL 135 APRIL 1970 BUCKLING COEFFICIENTS FOR SIMPLY SUPPORTED, FLAT, RECTANGULAR SANDWICH PANELS UNDER BIAXIAL COMPRESSION FOREST PRODUCTS LABORATORY, FOREST SERVICE
More informationDEFLECTION OF BEAMS WlTH SPECIAL REFERENCE TO SHEAR DEFORMATIONS
DEFLECTION OF BEAMS WlTH SPECIAL REFERENCE TO SHEAR DEFORMATIONS THE INFLUENCE OF THE FORM OF A WOODEN BEAM ON ITS STIFFNESS AND STRENGTHI (REPRINT FROM NATIONAL ADVISORY COMMITTEE FOR AERONAUTICS REPORT
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationCORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS
CORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS By Edmond P. Saliklis 1 and Robert H. Falk ABSTRACT: The weakness of existing relationships correlating offaxis modulus of elasticity
More informationELASTIC STAIBILITY CIF TUE FACINGS Of HAT SANDWICI1 PANELS WIASI SUBJECTED TO COMBINED EDGEWISE STRESSES
ELASTIC STAIBILITY CIF TUE FACINGS Of HAT SANDWICI1 PANELS WIASI SUBJECTED TO COMBINED EDGEWISE STRESSES Information Reviewed and Reaffirmed Aucust 1955 NFORMAtiON RE'4,E\AE.'L; n PE.117;9';f2,. This!Report
More informationExercise: concepts from chapter 8
Reading: Fundamentals of Structural Geology, Ch 8 1) The following exercises explore elementary concepts associated with a linear elastic material that is isotropic and homogeneous with respect to elastic
More informationCombined Stresses and Mohr s Circle. General Case of Combined Stresses. General Case of Combined Stresses con t. Twodimensional stress condition
Combined Stresses and Mohr s Circle Material in this lecture was taken from chapter 4 of General Case of Combined Stresses Twodimensional stress condition General Case of Combined Stresses con t The normal
More informationSEMM Mechanics PhD Preliminary Exam Spring Consider a twodimensional rigid motion, whose displacement field is given by
SEMM Mechanics PhD Preliminary Exam Spring 2014 1. Consider a twodimensional rigid motion, whose displacement field is given by u(x) = [cos(β)x 1 + sin(β)x 2 X 1 ]e 1 + [ sin(β)x 1 + cos(β)x 2 X 2 ]e
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More informationMINIMUM WEIGHT STRUCTURAL SANDWICH
U.S. DEPARTMENT OF AGRICULTURE FOREST SERVICE FOREST PRODUCTS LABORATORY MADISON, WIS. In Cooperation with the University of Wisconsin U.S.D.A. FOREST SERVICE RESEARCH NOTE Revised NOVEMBER 1970 MINIMUM
More informationri [11111 IlL DIRECTIONAL PROPERTIES Of GLASSFABRICBASE PLASTIC LAMINATE PANELS Of SIZES THAT DO NOT IBUCICLE (PQ1lAtVjr) No.
Supplement to DIRECTIONAL PROPERTIES Of GLASSFABRICBASE PLASTIC LAMINATE PANELS Of SIZES THAT DO NOT IBUCICLE (PQ1lAtVjr) No. 180313 November 1955 This Report is One of a Series issued hi Cooperation
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationTvestigated using the quadratic form of the TsaiWu strength theory [I].
Evaluation of Strength the TensorPolynomial Theory for Wood J. Y. L IU* Forest Products Laboratory, Forest Service U.S. Department of Agriculture, Madison, Wisconsin 53705 (Received October 10, 1983) (Revised
More informationChapter 3. Load and Stress Analysis. Lecture Slides
Lecture Slides Chapter 3 Load and Stress Analysis 2015 by McGraw Hill Education. This is proprietary material solely for authorized instructor use. Not authorized for sale or distribution in any manner.
More informationCORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS
CORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS By Edmond P. Saliklis 1 and Robert H. Falk 2 ABSTRACT: The weakness of existing relationships correlating offaxis modulus of elasticity
More informationEngineering Fracture Mechanics 74 (2007) Elsevier Ltd, doi: /j.engfracmech
Engineering Fracture Mechanics 74 (007) 771781 Elsevier Ltd, doi: 101016/j.engfracmech.006.06.015 A new fracture mechanics theory of orthotropic materials like wood T.A.C.M. van der Put, TUDelft, CiTG,
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationExample3. Title. Description. Cylindrical Hole in an Infinite MohrCoulomb Medium
Example3 Title Cylindrical Hole in an Infinite MohrCoulomb Medium Description The problem concerns the determination of stresses and displacements for the case of a cylindrical hole in an infinite elastoplastic
More informationLecture 8. Stress Strain in Multidimension
Lecture 8. Stress Strain in Multidimension Module. General Field Equations General Field Equations [] Equilibrium Equations in Elastic bodies xx x y z yx zx f x 0, etc [2] Kinematics xx u x x,etc. [3]
More informationSamantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2
Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationCHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES
CHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES * Governing equations in beam and plate bending ** Solution by superposition 1.1 From Beam Bending to Plate Bending 1.2 Governing Equations For Symmetric
More informationUNIT I Thin plate theory, Structural Instability:
UNIT I Thin plate theory, Structural Instability: Analysis of thin rectangular plates subject to bending, twisting, distributed transverse load, combined bending and inplane loading Thin plates having
More information[5] Stress and Strain
[5] Stress and Strain Page 1 of 34 [5] Stress and Strain [5.1] Internal Stress of Solids [5.2] Design of Simple Connections (will not be covered in class) [5.3] Deformation and Strain [5.4] Hooke s Law
More informationSTRENGTH AND STIFFNESS REDUCTION OF LARGE NOTCHED BEAMS
STRENGTH AND STIFFNESS REDUCTION OF LARGE NOTCHED BEAMS By Joseph F. Murphy 1 ABSTRACT: Four large glulam beams with notches on the tension side were tested for strength and stiffness. Using either bending
More informationS HEAR S TRENGTH IN P RINCIPAL P LANE OF W OOD
S HEAR S TRENGTH IN P RINCIPAL P LANE OF W OOD By Jen Y. Liu 1 and Lester H. Floeter 2 ABSTRACT: In this study, the writers used Tsai and Wu s tensor polynomial theory to rederive a formula originally
More information3D Elasticity Theory
3D lasticity Theory Many structural analysis problems are analysed using the theory of elasticity in which Hooke s law is used to enforce proportionality between stress and strain at any deformation level.
More informationPlane and axisymmetric models in Mentat & MARC. Tutorial with some Background
Plane and axisymmetric models in Mentat & MARC Tutorial with some Background Eindhoven University of Technology Department of Mechanical Engineering Piet J.G. Schreurs Lambèrt C.A. van Breemen March 6,
More informationLecture 15 Strain and stress in beams
Spring, 2019 ME 323 Mechanics of Materials Lecture 15 Strain and stress in beams Reading assignment: 6.1 6.2 News: Instructor: Prof. Marcial Gonzalez Last modified: 1/6/19 9:42:38 PM Beam theory (@ ME
More informationChapter Two: Mechanical Properties of materials
Chapter Two: Mechanical Properties of materials Time : 16 Hours An important consideration in the choice of a material is the way it behave when subjected to force. The mechanical properties of a material
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationEmpirical Prediction of Shear Modulus and Young's Modulus of Plywood Panels
Empirical Prediction of Shear Modulus and Young's Modulus of Plywood Panels By Edmond P. Saliklis Assistant Professor of Civil and Environmental Engineering 3 Alumni Hall of Engineering Lafayette College,
More informationMarch No In Cooperation with the University of Wisconsin
March 1956 No. In Cooperation with the University of Wisconsin STRESSES IN WOOD MEMBERS SUBJECTED TO COMBINED COLUMN AND BEAM ACTION.* J. A. NEWLIN and G. W. TRAYER. INTRODUCTION. This publication is one
More informationCHAPER THREE ANALYSIS OF PLANE STRESS AND STRAIN
CHAPER THREE ANALYSIS OF PLANE STRESS AND STRAIN Introduction This chapter is concerned with finding normal and shear stresses acting on inclined sections cut through a member, because these stresses may
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationPURE BENDING. If a simply supported beam carries two point loads of 10 kn as shown in the following figure, pure bending occurs at segment BC.
BENDING STRESS The effect of a bending moment applied to a crosssection of a beam is to induce a state of stress across that section. These stresses are known as bending stresses and they act normally
More informationFLEXURE OF STRUCTURAL SANDWICH CONSTRUCTION
FLEXURE OF STRUCTURAL SANDWICH CONSTRUCTION December 1951 INFORMATION REVIEWED AND REAFFIRMED 1958 LOAN COPY Please return to: Wood Engineering Research Forest Products Laboratory Madison, Wisconsin 53705
More informationSymmetric Bending of Beams
Symmetric Bending of Beams beam is any long structural member on which loads act perpendicular to the longitudinal axis. Learning objectives Understand the theory, its limitations and its applications
More informationChapter 12. Static Equilibrium and Elasticity
Chapter 12 Static Equilibrium and Elasticity Static Equilibrium Equilibrium implies that the object moves with both constant velocity and constant angular velocity relative to an observer in an inertial
More informationTHE BENDING STIFFNESSES OF CORRUGATED BOARD
AMDVol. 145/MDVol. 36, Mechanics of Cellulosic Materials ASME 1992 THE BENDING STIFFNESSES OF CORRUGATED BOARD S. Luo and J. C. Suhling Department of Mechanical Engineering Auburn University Auburn,
More informationMechanics of Earthquakes and Faulting
Mechanics of Earthquakes and Faulting www.geosc.psu.edu/courses/geosc508 Surface and body forces Tensors, Mohr circles. Theoretical strength of materials Defects Stress concentrations Griffith failure
More informationTentamen/Examination TMHL61
Avd Hållfasthetslära, IKP, Linköpings Universitet Tentamen/Examination TMHL61 Tentamen i Skademekanik och livslängdsanalys TMHL61 lördagen den 14/10 2000, kl 812 Solid Mechanics, IKP, Linköping University
More informationProperties of surfaces II: Second moment of area
Properties of surfaces II: Second moment of area Just as we have discussing first moment of an area and its relation with problems in mechanics, we will now describe second moment and product of area of
More informationTHEORY OF PLATES AND SHELLS
THEORY OF PLATES AND SHELLS S. TIMOSHENKO Professor Emeritus of Engineering Mechanics Stanford University S. WOINOWSKYKRIEGER Professor of Engineering Mechanics Laval University SECOND EDITION MCGRAWHILL
More informationTHEORETICAL DESIGN OF A NAILED OR BOLTED JOINT UNDER LATERAL LOAD 1. Summary
THEORETICAL DESIGN OF A NAILED OR BOLTED JOINT UNDER LATERAL LOAD 1 BY EDWARD W. KUENZI, 2 Engineer Forest Products Laboratory,3 Forest Service U. S. Department of Agriculture Summary This report presents
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationNORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.
NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric
More information3 2 6 Solve the initial value problem u ( t) 3. a If A has eigenvalues λ =, λ = 1 and corresponding eigenvectors 1
Math Problem a If A has eigenvalues λ =, λ = 1 and corresponding eigenvectors 1 3 6 Solve the initial value problem u ( t) = Au( t) with u (0) =. 3 1 u 1 =, u 1 3 = b True or false and why 1. if A is
More informationPurpose of this Guide: To thoroughly prepare students for the exact types of problems that will be on Exam 3.
ES230 STRENGTH OF MTERILS Exam 3 Study Guide Exam 3: Wednesday, March 8 th inclass Updated 3/3/17 Purpose of this Guide: To thoroughly prepare students for the exact types of problems that will be on
More informationTorsion of Solid Sections. Introduction
Introduction Torque is a common load in aircraft structures In torsion of circular sections, shear strain is a linear function of radial distance Plane sections are assumed to rotate as rigid bodies These
More informationMechanical Engineering Ph.D. Preliminary Qualifying Examination Solid Mechanics February 25, 2002
student personal identification (ID) number on each sheet. Do not write your name on any sheet. #1. A homogeneous, isotropic, linear elastic bar has rectangular cross sectional area A, modulus of elasticity
More informationBasic Equations of Elasticity
A Basic Equations of Elasticity A.1 STRESS The state of stress at any point in a loaded bo is defined completely in terms of the nine components of stress: σ xx,σ yy,σ zz,σ xy,σ yx,σ yz,σ zy,σ zx,andσ
More information7.3 Design of members subjected to combined forces
7.3 Design of members subjected to combined forces 7.3.1 General In the previous chapters of Draft IS: 800 LSM version, we have stipulated the codal provisions for determining the stress distribution in
More information5. STRESS CONCENTRATIONS. and strains in shafts apply only to solid and hollow circular shafts while they are in the
5. STRESS CONCENTRATIONS So far in this thesis, most of the formulas we have seen to calculate the stresses and strains in shafts apply only to solid and hollow circular shafts while they are in the elastic
More informationEFFECTIVE THICKNESS OF PAPER: APPRAISAL AND FURTHER DEVELOPMENT
EFFECTIVE THICKNESS OF PAPER: APPRAISAL AND FURTHER DEVELOPMENT USDA FOREST SERVICE RESEARCH PAPER FPL 287 1977 U.S. DEPARTMENT OF AGRICULTURE FOREST SERVICE FOREST PRODUCTS LABORATORY MADISON, WIS. Abstract
More informationTORSIONAL RIGIDITY OF WOOD COMPOSITE IJOISTS Daniel Hindman. Harvey B. Manbeck. John J. Janowiak
TORSIONAL RIGIDITY OF WOOD COMPOSITE IJOISTS Daniel Hindman Assistant Professor Department of Wood Science and Forest Products Virginia Polytechnic Institute and State University Brooks Forest Products
More informationExample 3.7 Consider the undeformed configuration of a solid as shown in Figure 3.60.
162 3. The linear 3D elasticity mathematical model The 3D elasticity model is of great importance, since it is our highest order hierarchical model assuming linear elastic behavior. Therefore, it provides
More informationME 2570 MECHANICS OF MATERIALS
ME 2570 MECHANICS OF MATERIALS Chapter III. Mechanical Properties of Materials 1 Tension and Compression Test The strength of a material depends on its ability to sustain a load without undue deformation
More informationSTRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS
1 UNIT I STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define: Stress When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More information7.6 Stress in symmetrical elastic beam transmitting both shear force and bending moment
7.6 Stress in symmetrical elastic beam transmitting both shear force and bending moment à It is more difficult to obtain an exact solution to this problem since the presence of the shear force means that
More information1.105 Solid Mechanics Laboratory Fall 2003
1.105 Solid Mechanics Laboratory Fall 200 Experiment 7 Elastic Buckling. The objectives of this experiment are To study the failure of a truss structure due to local buckling of a compression member. To
More informationEVALUATION OF MODULUS OF RIGIDITY BY DYNAMIC PLATE SHEAR TESTING Tetsuya Nakao. and Takeshi Okano
EVALUATION OF MODULUS OF RIGIDITY BY DYNAMIC PLATE SHEAR TESTING Tetsuya Nakao Graduate Student Present address: Department of Forestry Faculty of Agriculture Shimane University Matsue 690, Japan and Takeshi
More informationMechanics of Materials Primer
Mechanics of Materials rimer Notation: A = area (net = with holes, bearing = in contact, etc...) b = total width of material at a horizontal section d = diameter of a hole D = symbol for diameter E = modulus
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More informationMECHANICS OF MATERIALS
2009 The McGrawHill Companies, Inc. All rights reserved. Fifth SI Edition CHAPTER 3 MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf David F. Mazurek Torsion Lecture Notes:
More information3 Shearing stress. 3.1 Introduction
3 Shearing stress 3.1 Introduction In Chapter 1 we made a study of tensile and compressive stresses, which we called direct stresses. There is another type of stress which plays a vital role in the behaviour
More informationStresses in Curved Beam
Stresses in Curved Beam Consider a curved beam subjected to bending moment M b as shown in the figure. The distribution of stress in curved flexural member is determined by using the following assumptions:
More informationME Final Exam. PROBLEM NO. 4 Part A (2 points max.) M (x) y. z (neutral axis) beam crosssec+on. 20 kip ft. 0.2 ft. 10 ft. 0.1 ft.
ME 323  Final Exam Name December 15, 2015 Instructor (circle) PROEM NO. 4 Part A (2 points max.) Krousgrill 11:30AM12:20PM Ghosh 2:303:20PM Gonzalez 12:301:20PM Zhao 4:305:20PM M (x) y 20 kip ft 0.2
More informationNAME: Given Formulae: Law of Cosines: Law of Sines:
NME: Given Formulae: Law of Cosines: EXM 3 PST PROBLEMS (LESSONS 21 TO 28) 100 points Thursday, November 16, 2017, 7pm to 9:30, Room 200 You are allowed to use a calculator and drawing equipment, only.
More informationACCURATE FREE VIBRATION ANALYSIS OF POINT SUPPORTED MINDLIN PLATES BY THE SUPERPOSITION METHOD
Journal of Sound and Vibration (1999) 219(2), 265 277 Article No. jsvi.1998.1874, available online at http://www.idealibrary.com.on ACCURATE FREE VIBRATION ANALYSIS OF POINT SUPPORTED MINDLIN PLATES BY
More informationBOOK OF COURSE WORKS ON STRENGTH OF MATERIALS FOR THE 2 ND YEAR STUDENTS OF THE UACEG
BOOK OF COURSE WORKS ON STRENGTH OF MATERIALS FOR THE ND YEAR STUDENTS OF THE UACEG Assoc.Prof. Dr. Svetlana LilkovaMarkova, Chief. Assist. Prof. Dimitar Lolov Sofia, 011 STRENGTH OF MATERIALS GENERAL
More informationQUESTION BANK DEPARTMENT: CIVIL SEMESTER: III SUBJECT CODE: CE2201 SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A
DEPARTMENT: CIVIL SUBJECT CODE: CE2201 QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A (2 Marks) 1. Define longitudinal strain and lateral strain. 2. State
More informationSmart Materials, Adaptive Structures, and Intelligent Mechanical Systems
Smart Materials, Adaptive Structures, and Intelligent Mechanical Systems Bishakh Bhattacharya & Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 19 Analysis of an Orthotropic Ply References
More informationUNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationSTRESSEDSKIN PANEL DEFLECTIONS AND STRESSES USDA FOREST SERVICE RESEARCH PAPER
STRESSEDSKIN PANEL DEFLECTIONS AND STRESSES USDA FOREST SERVICE RESEARCH PAPER FPL 251 1975 U. S. DEPARTMENT OF AGRICULTURE FOREST SERVICE FOREST PRODUCTS LABORATORY MADISON, WISCONSIN ABSTRACT This paper
More informationBUCKLING COEFFICIENTS FOR SANDWICH CYLINDERS OF FINITE LENGTH UNDER UNIFORM EXTERNAL LATERAL PRESSURE
U.S. DEPARTMENT OF AGRICULTURE FOREST SERVICE FOREST PRODUCTS LABORATORY MADlSON, WIS. In Cooperation with the University of Wisconsin U. S. FOREST SERVICE RESEARCH NOTE FPL0104 SEPTEMBER 1965 BUCKLING
More information(48) CHAPTER 3: TORSION
(48) CHAPTER 3: TORSION Introduction: In this chapter structural members and machine parts that are in torsion will be considered. More specifically, you will analyze the stresses and strains in members
More informationIMPACT OF LAMINATE DIRECTIONS ON IN PLANE SHEAR STIFFNESS OF CROSS LAMINATED TIMBER
IMPACT OF LAMINATE DIRECTIONS ON IN PLANE SHEAR STIFFNESS OF CROSS LAMINATED TIMBER Turesson, J. 1 & Ekevad, M. 2 ABSTRACT Twentythree finite element models of crosslaminated timber (CLT) with different
More information6.1 Formulation of the basic equations of torsion of prismatic bars (St. Venant) Figure 6.1: Torsion of a prismatic bar
Module 6 Torsion Learning Objectives 6.1 Formulation of the basic equations of torsion of prismatic bars (St. Venant) Readings: Sadd 9.3, Timoshenko Chapter 11 e e 1 e 3 Figure 6.1: Torsion of a prismatic
More informationEDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES AND APPLICATIONS NQF LEVEL 3 OUTCOME 1  LOADING SYSTEMS TUTORIAL 3 LOADED COMPONENTS
EDEXCEL NATIONAL CERTIICATE/DIPLOMA MECHANICAL PRINCIPLES AND APPLICATIONS NQ LEVEL 3 OUTCOME 1  LOADING SYSTEMS TUTORIAL 3 LOADED COMPONENTS 1. Be able to determine the effects of loading in static engineering
More informationModule4. Mechanical Properties of Metals
Module4 Mechanical Properties of Metals Contents ) Elastic deformation and Plastic deformation ) Interpretation of tensile stressstrain curves 3) Yielding under multiaxial stress, Yield criteria, Macroscopic
More informationA STUDY OF THE STRENGTH OF SHORT AND INTERMEDIATE WOOD COLUMNS BY EXPERIMENTAL AND ANALYTICAL METHODS
UNITED STATES DEPARTMENT OF AGRICULTURE. FOREST SERVICE. FOREST PRODUCTS LABORATORY. MADISON, WIS A STUDY OF THE STRENGTH OF SHORT AND INTERMEDIATE WOOD COLUMNS BY EXPERIMENTAL AND ANALYTICAL METHODS January
More informationARTICLE A8000 STRESSES IN PERFORATED FLAT PLATES
ARTICLE A8000 STRESSES IN PERFORATED FLAT PLATES Delete endnote 18, which says "Express metric values in exponential form" A8100 INTRODUCTION A8110 SCOPE (a) This Article contains a method of analysis
More informationMechanics in Energy Resources Engineering  Chapter 5 Stresses in Beams (Basic topics)
Week 7, 14 March Mechanics in Energy Resources Engineering  Chapter 5 Stresses in Beams (Basic topics) KiBok Min, PhD Assistant Professor Energy Resources Engineering i Seoul National University Shear
More informationVYSOKÁ ŠKOLA BÁŇSKÁ TECHNICKÁ UNIVERZITA OSTRAVA
VYSOKÁ ŠKOLA BÁŇSKÁ TECHNICKÁ UNIVERZITA OSTRAVA FAKULTA METALURGIE A MATERIÁLOVÉHO INŽENÝRSTVÍ APPLIED MECHANICS Study Support Leo Václavek Ostrava 2015 Title:Applied Mechanics Code: Author: doc. Ing.
More informationAdvanced Structural Analysis EGF Section Properties and Bending
Advanced Structural Analysis EGF316 3. Section Properties and Bending 3.1 Loads in beams When we analyse beams, we need to consider various types of loads acting on them, for example, axial forces, shear
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationSolid Mechanics Chapter 1: Tension, Compression and Shear
Solid Mechanics Chapter 1: Tension, Compression and Shear Dr. Imran Latif Department of Civil and Environmental Engineering College of Engineering University of Nizwa (UoN) 1 Why do we study Mechanics
More information